EXPERIMENTAL EVALUATION OF SHEAR STRENGTH OF WOVEN WEBBINGS


 Alan Nicholson
 1 years ago
 Views:
Transcription
1 EXPERIMENTAL EVALUATION OF SHEAR STRENGTH OF WOVEN WEBBINGS Kevin L. Peil +, Ever J. Barbero +, Eduardo M. Sosa* + Department of Mechanical and Aerospace Engineering, West Virginia University (WVU), Morgantown, West Virginia, USA *Department of Civil and Environmental Engineering, West Virginia University (WVU), Morgantown, West Virginia, USA The development of Finite Element Models (FEM) of inflatable structures made from woven webbings used to seal conduits and large pipes with irregular shapes requires not only the typical material properties such as modulus of elasticity, axial strength, density, and Poisson's ratio, but also an estimation of the shear behavior to account for the drapeability of the inflatable necessary to conform to the irregularities of the section to be sealed. Because the fibers in woven webbings are not continuous along the two principle directions, a priori it is not possible to calculate analytically the shear properties based on the fiber elastic modulus and Poisson s ratio. Due to this limitation, mechanical testing is necessary to determine the shear behavior. An experimental methodology for determining the shear characteristics of woven webbings is proposed. Experimental methods are developed for testing the materials using the denominated "picture frame" designed to produce a shearing effect from an axial force. These frames allow the materials to be stressed biaxially prior to the shear testing to observe the shear performance under similar axial stress states, which will be seen in the material for specific applications. Testing yields load and displacement data, which can be used to determine the shear modulus as a function of the materials angular displacement. The Department of Homeland Security, Science and Technology Directorate, Infrastructure Protection and Disaster Management Division provided funding support for this research. 1. INTRODUCTION The shear characteristics of fabrics have been analyzed in a number of ways ranging from mathematical models, which predict the material behavior based on fiber geometry and friction coefficients, to mechanical testing, which directly measures a materials bulk resistance to shear deformation [1][2]. The shear mechanisms influence the draping and pliability of a fabric and determine the ability of the material to conform to a three dimensional surface [1]. The ability of a fabric to conform to a doublecurvature surface depends mainly on the inplane shear behavior [3]. Because the fibers within a webbing are not continuous and are not connected along any two principle directions, the materials cannot be considered isotropic or homogeneous. These types of micromaterials can also display nonlinear and unpredictable behavior under multiple stress states. Because of this, a theoretical analysis can become very complex or impossible and experimental determination of the material behavior becomes necessary. The shear properties of webbings will be dependent on the biaxial state of stress, which the material will be under. The material must be tested in a manner where the tensile and shear forces can be applied simultaneously [4].
2 Material Selection Two materials, nylon and Vectran, HT, were used to categorize the shear behavior of the woven outer layer of the inflatable structure being analyzed in the FEM. The use of two materials was necessary due to the limited supply of Vectran available for testing. The nylon webbings that were used had the same width and thickness as Vectran and similar coefficients of friction. The principle difference between the two materials is the ultimate tensile strength. A table summarizing the key properties of the two materials is shown in Table 1. Because the mechanisms of shear are a function of weave pattern, friction coefficient, and pretensioning, and are roughly independent of the tensile strength of the individual fibers [1], conclusions on the shear characteristics of the outer layer of the inflatable structure could be drawn from tests run using both materials. Table 1: Material properties of Nylon and Vectran HT webbings Width Thickness Coefficient of Ultimate Tensile friction Strength Weave pattern Nylon 2 inches 0.1 inch ~0.5 7,000 lb herringbone Vectran 2 inches 0.1 inch ~0.5 24,000 lb herringbone Material Preparation Twelve strips were initially cut from a bulk roll of material to be woven together to form a representative volume element (RVE) of a section of the inflatable structure being analyzed. The weave pattern used was a square weave. Strips were cut 27 inches in length to allow for attachment to the picture frame shear test stand and pretensioning pulley system. A smaller RVE could have been used to measure the shear behavior of the material under small angular displacements (020 degrees), however jamming of the fibers and wrinkling of the material, which occurred at large angular displacements (2036 degrees), would not have been observable. Samples were prepared under dry conditions at ambient air temperatures. Picture Frame Shear Test Stand Preparation Figure 2: CAD image of picture frame shear test stand A picture frame shear test stand was used to apply the shearing loads to the sample during testing. A computeraided design (CAD) image of the frame that was built is shown in figure 2. The arms of the frame measured nineteen inches in length, two inches wide and one inch thick. The design of the frame allowed the material to be pretensioned along each principle direction prior to attachment, permitting the measurement of shear under a biaxial state of stress. While in the frame, the strips of material were held in place using a dead man system, which uses the materials self friction to hold the bottom of each strip in the frame and a steel plate secured with bolts to hold the top of each strip. Because of the design of the frame, while the material was being sheared, the
3 distance between any two colinear connection points would remain equidistant. This allowed the biaxial stress state in the material to remain constant during testing. The frame was constructed using halfinch thick 304 stainless steel plate. The pivot bearings were made from smoothed, oneinch diameter, solid stainlesssteel shafts cut four inches long. Between the steel arm plates were thin Vectran shims used to ensure uniform contact along the length of the frame. 2. EXPERIMENTATION Material PreTensioning Pretensioning of the webbing strips began with attachment of the bottom of each strip to the shear test frame using a dead man gripping method. Six strips of webbing material were laid side by side on top of the disassembled shear test frame, perpendicular to the length of the bottom arm with two inches of overhang. The overhang of each strip was then folded over top of a halfinch, plain carbon steel rod and held in place using four staples. Once all six webbings were folded over the rod, Vectran shims were laid across the length of the arm to assure even contact with the steel holding plate. The top of the shear test frame arm was then attached over the folded webbings. The top of each webbing strip was then attached to a specially designed pretensioning pulley system. The pulley system was comprised of three twoinch diameter wheels spaced four inches apart from one another. The wheels were mounted on a set of steel plates, which allowed independent movement of each wheel relative to one another. Steel cables with attached mounting plates were then wrapped over the pulleys for attachment to the top end of each webbing strip. Due to the design of the pulley system and the method of attachment, when a tensile load was applied to the top arm of the system the load would be equally distributed to each webbing, resulting in a uniform stress across the width of the sample. Figure 3: Vectran sample attached to pulley system and frame for pretensioning Figure 3: Vectran sample attached to pulley system and frame for pretensioning To apply the required pretensioning load, the pulley system and shear test frame were connected to an Instron HDX1000 tensile test machine. Connections were made to the machine via two oneinch diameter steel shafts, which were attached to solid steel blocks held in place using the machines hydraulic wedge grips. The pulley system was initially lifted into place and secured to the top bolt. The bottom crosshead on the tensile test machine was then raised into position to attach to the bottom of the shear test frame. An image of the pulley system and shear test frame attached to the tensile test machine with Vectran webbings at the pretensioning stage can be seen in figure 3.After attachment to the tensile test machine, the system was tensioned to approximately 600 pounds per webbing and held at this load for 10 minutes to allow for stress relaxation within the system. A top holding plate was secured to the ends of the webbings using 12 bolts. Attachment of the holding plate required all components to be held tightly in place using four Cclamps and wedges.
4 Had the material not been held tightly in place, as the fibers were broken by the drill to produce bolt holes, they would have been pulled down within the frame resulting in a local loss of tension in the vicinity of each bolt. This would have resulted in prematuree wrinkling of the sample as well as an overall inaccuracy in the representation of the material layer that was to be modeled. Once attachment had been completed, the shear test frame and pulley system were removed from the tensile test machine and the excess material connecting the shear test frame to the pulley system was cut. The procedure was repeated for the set of perpendicular webbings resulting in a representative volume element of the woven outer layer of the inflatable structure being held in place within the shear test frame under a uniform biaxial state of stress. Shear Testing of the Prepared Sample After sample preparation and detachment from the pulley system, the shear test frame was reattached to the tensile test machine from two pivot points on opposite corners of the frame. Using Instron s Partner software, a program was written that would move the top bearing of the shear frame upward at a rate of 0.02 inches per second. The program recorded crosshead displacement, load on the frame, and time. The displacement of the top of the frame resulted in the material being deformed into a diamond shape, shearing the material as the frame was displaced. From the data collected, the nominal shear stress in the material and the angular displacement of the fibers could be calculated. Each sample was sheared five times to an angular displacement of approximately 36 degrees. Tests were stopped when large amounts of wrinkling were observed. An image of a sheared sample of nylon is shown in figure 4. Figure 4: Images of Nylon sample under varying angles of shear deformation 3. RESULTS Analysis of shear was done in a manner that would yield results usable within the FEM of the inflatable structure being investigated. The model was developed using Abaqus software, which requires an input plot of nominal shear stress versus fiber change in angle [5]. As such, this information was calculated and plotted based on the deformation of the frame and the required load to cause the deformation. After plotting the results from each test, the values were averaged to form a single representative plot of nominal shear stress versus fiber change in angle.
5 Each test had a slight difference in the amount of measured preload after sample attachment. This was due to fiber slippage caused by the holes that were drilled for attachment and tightening of the interface between the top steel holding plates and the top arm of the shear test frame. The recorded initial preloads and loads after attachment for each of the principle directions are supplied in table 2. The experimental setup of the tests was seen to be a major factor in the accuracy of each trial. Sample placement within the frame must be exact to assure the material is sheared properly. All connections along the frame for securing the webbing materials must be made while minimizing any fiber slippage to maintain a uniform preload along the length of the sample. Material was monitored during testing to assure damage was not induced as a result of over deformation. Table 2: Material Preload in the two principle directions Sample Initial Preload (direction 1) Load after attachment (direction 1) Load per webbing Initial Preload (direction 2) Load after attachment (direction 2) Load per webbing Sample 1 (Nylon) Sample 2 (Nylon) Sample 3 (Nylon) Sample 4 (Nylon) Sample 5 (Vectran) 4000 lb 2860 lb 477 lb 4000 lb 2780 lb 463 lb 4000 lb 3180 lb 530 lb 4000 lb 3264 lb 544 lb 4000 lb 3280 lb 547 lb 4000 lb 3411 lb 569 lb 4000 lb 3500 lb 583 lb 4000 lb 3500 lb 583 lb 4900 lb 4174 lb 696 lb 4900 lb 4500 lb 750 lb The frame geometry, deflection, and data from each test were used to calculate webbing change in angle. Knowing that the initial distance between two opposite pivot points on the frame was inches in the undeformed (i.e., square) configuration and that the side length of each arm between each pivot point was 19 inches, equation 1 could be used to determine the change in angle of the webbings as a function of the crosshead displacement at any given time. Figure 5 shows a schematic of the information needed from the tests frame to perform the calculations.
6 L F w w θ Figure 5: Schematic of picture frame shear test pertinent information The nominal shear stress (T 12 ) in the material is calculated as a function of material thickness, width of the sample, applied load, and angular displacement. Nominal shear stress was calculated using equation 2. Equation 1: θ = 90 2 cos. F Equation 2: T = Where L is the displacement of the tensile test machine crosshead, F is the applied load to the frame as measured by the tensile test machine, t is the material thickness of.2 inch, w is the edge width of the sample (12 inches) and θ is the angular displacement of the webbings. Data produced by the tensile test machine were reduced using MATLAB, producing figure 6 showing the results from each trial.
7 Figure 6: Complete results of each trial. A more compact and easily understood plot was produced by taking the average of all trials for each test. Best fit curves were mathematically forced through the origin in accordance with experimental observations. A plot of the averages from each test can be seen in Figure 7. Figure 7: Averaged results for each test From the above results, points can be chosen to represent key elements of the curve that define the shear behavior. For the FEA model, 12 points were used, each separated by three degrees. There are four shearing mechanisms that can be observed from the results. Under angular displacements between zero and 2.5 degrees, the deformation of the material is too small to overcome the friction between the strips of webbing. As such, the material acts as a rigid body
8 and the slope representing the shear modulus is large. Between 2.5 and 20 degrees of angular displacement, there is yarn slippage at the intersection and elastic bending resulting in the flattening of the curve. At angles above 20 degrees, there is jamming and wrinkling within the material requiring larger shear stresses to produce the displacements. The final plot used to define the material shear behavior can be seen in figure 8. Figure 8: Data points defining the material shear behavior for Vectran and Nylon The tests showed a large amount of variability between samples, speculatively due to the differences in preload between tests. Fiber micromechanic behavior was an additional source of variability, due to the differences in tension across the width of the sample caused by fiber slippage during sample attachment. Future work will be done to visually map the individual changes in webbing angle using digital image correlation, which will then be compared with equation 1 to determine the accuracy of the assumption that the webbing change in angle is equal to that of the frame. As shear deformation angle increases and jamming of the material occurs, angular displacements of the webbings in the vicinity of the intersection points were seen to be larger than that of the bulk of the surface. These intersections will require further study and evaluation to determine the stress state at these points. 4. CONCLUSIONS The use of a picture frame shear test stand was seen as a viable method for evaluating the shear characteristics of a woven material. The ability to pretension a fabric sample prior to shear testing is required due to the nature of the fiber interactions as the sample is displaced. Experimental measurement of the shear performance of fabrics is required as no method for accurately calculating the behavior is available. Tests must be performed under the same state of
9 biaxial stress, which will be seen by the material when in use. Friction between fibers was seen to be the primary mechanism for shear resistance. Evaluation of the results indicates that the outer layer of the inflatable structure will show little resistance to shear deformation as is required for the structure to conform to irregularities within the conduits it will be housed within. 5. REFERENCES 1. Grosberg, P., Park, B.J., The mechanical properties of woven fabrics. Part V. The initial modulus and the frictional restraint in shearing of plain weave fabrics. Textile Res J 1966;36: Domskiene, J., Strazdien, E., Investigation of fabric shear behavior. Fibres &Textiles in Eastern Europe April/June 2005, Vol.13 No.2(50) 3. Potluri, P., Ciurezu, D. Young, R. Biaxial shear testing of textile performs for formability analysis. 16 th International Conference on Composite Materials Basset, R., Postle, R., Experimental methods for measuring fabric mechanical properties: A review and analysis. Textile Res J. 69(11), (1999) 5. L. Dong, C. Lekakou and M. G. Bader, Processing of Composites: Simulations of the Draping of Fabrics with Updated Material Behaviour Law. Journal of Composite Materials : Abaqus 6.8. User Manual 7. Sun, H., Pan, N., Shear deformation analysis for woven fabrics. Composite Structures 67(2005)
Measurement of mesoscale deformations for modelling textile composites
CompTest 2004 Measurement of mesoscale deformations for modelling textile composites P Potluri, D A Perez Ciurezu, R Ramgulam Textile Composites Group University of Manchester Institute of Science & Technology
More informationDRAPING SIMULATION. Recent achievements and future trends. Dr. Sylvain Bel LGCIE University Lyon 1
DRAPING SIMULATION Recent achievements and future trends 1 Dr. Sylvain Bel LGCIE University Lyon 1 2 DRAPING SIMULATION Why? How? What? DRAPING SIMULATION WHY? Clamps Punch Fabric Die 1 2 Resin 3 4 Fig.
More informationTuesday, February 11, Chapter 3. Load and Stress Analysis. Dr. Mohammad Suliman Abuhaiba, PE
1 Chapter 3 Load and Stress Analysis 2 Chapter Outline Equilibrium & FreeBody Diagrams Shear Force and Bending Moments in Beams Singularity Functions Stress Cartesian Stress Components Mohr s Circle for
More information[5] Stress and Strain
[5] Stress and Strain Page 1 of 34 [5] Stress and Strain [5.1] Internal Stress of Solids [5.2] Design of Simple Connections (will not be covered in class) [5.3] Deformation and Strain [5.4] Hooke s Law
More informationFLEXIBILITY METHOD FOR INDETERMINATE FRAMES
UNIT  I FLEXIBILITY METHOD FOR INDETERMINATE FRAMES 1. What is meant by indeterminate structures? Structures that do not satisfy the conditions of equilibrium are called indeterminate structure. These
More informationBioMechanics and BioMaterials Lab (BME 541) Experiment #5 Mechanical Prosperities of Biomaterials Tensile Test
BioMechanics and BioMaterials Lab (BME 541) Experiment #5 Mechanical Prosperities of Biomaterials Tensile Test Objectives 1. To be familiar with the material testing machine(810le4) and provide a practical
More informationElastic Properties of Solids (One or two weights)
Elastic properties of solids Page 1 of 8 Elastic Properties of Solids (One or two weights) This is a rare experiment where you will get points for breaking a sample! The recommended textbooks and other
More informationExperiment Two (2) Torsional testing of Circular Shafts
Experiment Two (2) Torsional testing of Circular Shafts Introduction: Torsion occurs when any shaft is subjected to a torque. This is true whether the shaft is rotating (such as drive shafts on engines,
More informationSHEAR TENSION COUPLING IN BIAXIAL BIAS EXTENSION TESTS
SHER TENSION COUPLING IN IXIL IS EXTENSION TESTS P. Harrison *, P. Potluri Department of Mechanical Engineering, James Watt uilding (South), University of Glasgow, Glasgow G 8QQ, U.K. p.harrison@mech.gla.ac.uk
More informationSamantha Ramirez, MSE. Stress. The intensity of the internal force acting on a specific plane (area) passing through a point. F 2
Samantha Ramirez, MSE Stress The intensity of the internal force acting on a specific plane (area) passing through a point. Δ ΔA Δ z Δ 1 2 ΔA Δ x Δ y ΔA is an infinitesimal size area with a uniform force
More informationMembers Subjected to Torsional Loads
Members Subjected to Torsional Loads Torsion of circular shafts Definition of Torsion: Consider a shaft rigidly clamped at one end and twisted at the other end by a torque T = F.d applied in a plane perpendicular
More informationChapter 12. Static Equilibrium and Elasticity
Chapter 12 Static Equilibrium and Elasticity Static Equilibrium Equilibrium implies that the object moves with both constant velocity and constant angular velocity relative to an observer in an inertial
More informationEquilibrium & Elasticity
PHYS 101 Previous Exam Problems CHAPTER 12 Equilibrium & Elasticity Static equilibrium Elasticity 1. A uniform steel bar of length 3.0 m and weight 20 N rests on two supports (A and B) at its ends. A block
More informationLab Exercise #5: Tension and Bending with Strain Gages
Lab Exercise #5: Tension and Bending with Strain Gages Prelab assignment: Yes No Goals: 1. To evaluate tension and bending stress models and Hooke s Law. a. σ = Mc/I and σ = P/A 2. To determine material
More informationContact pressure distribution in joints formed by Vband clamps Simon M Barrans 1,a, Goodarz Khodabakhshi 1,b and Qiang Xu 1,c
Contact pressure distribution in joints formed by Vband clamps Simon M Barrans 1,a, Goodarz Khodabakhshi 1,b and Qiang Xu 1,c 1 School of Computing and Engineering, University of Huddersfield, Queensgate,
More informationINSPIRE GK12 Lesson Plan. Elastic Deformation of Materials: An Investigation of Hooke s Law Length of Lesson
Lesson Title Elastic Deformation of Materials: An Investigation of Hooke s Law Length of Lesson 1.5 hours Created By Justin Warren Subject Physics Grade Level 1112 State Standards Physics: 1 c, d, f;
More informationMicromeso draping modelling of noncrimp fabrics
Micromeso draping modelling of noncrimp fabrics Oleksandr Vorobiov 1, Dr. Th. Bischoff 1, Dr. A. Tulke 1 1 FTA Forschungsgesellschaft für Textiltechnik mbh 1 Introduction Noncrimp fabrics (NCFs) are
More informationSize Effects In the Crushing of Honeycomb Structures
45th AIAA/ASME/ASCE/AHS/ASC Structures, Structural Dynamics & Materials Conference 1922 April 2004, Palm Springs, California AIAA 20041640 Size Effects In the Crushing of Honeycomb Structures Erik C.
More informationAn Analytical Study of Initial Shear Behavior of Plain Woven Hybrid Fabrics
JOURNAL OF TEXTILES AND POLYMERS, VOL. 4, NO., JANUARY 206 9 An Analytical Study of Initial Shear Behavior of Plain Woven Hybrid Fabrics Majid TehraniDehkor and Hooshang Nosraty Abstract During recent
More informationMULTISCALE MODELLING OF FIBRE BUNDLES
THE 19 TH INTERNATIONAL CONFERENCE ON COMPOSITE MATERIALS MULTISCALE MODELLING OF FIBRE BUNDLES N. D. Chakladar 1, P. Mandal 1 *, P. Potluri 2 1 School of Mechanical, Aerospace and Civil Engineering,
More informationBIAS EXTENSION TEST STANDARD
BIAS EXTENSION TEST STANDARD Xiongqi Peng and Jian Cao Advanced Materials Processing Laboratory Department of Mechanical Engineering Northwestern University Evanston, IL August 2003 For Internal Use 1.
More informationCONNECTION DESIGN. Connections must be designed at the strength limit state
CONNECTION DESIGN Connections must be designed at the strength limit state Average of the factored force effect at the connection and the force effect in the member at the same point At least 75% of the
More informationNAME: Given Formulae: Law of Cosines: Law of Sines:
NME: Given Formulae: Law of Cosines: EXM 3 PST PROBLEMS (LESSONS 21 TO 28) 100 points Thursday, November 16, 2017, 7pm to 9:30, Room 200 You are allowed to use a calculator and drawing equipment, only.
More informationInitial Stress Calculations
Initial Stress Calculations The following are the initial hand stress calculations conducted during the early stages of the design process. Therefore, some of the material properties as well as dimensions
More informationProblem " Â F y = 0. ) R A + 2R B + R C = 200 kn ) 2R A + 2R B = 200 kn [using symmetry R A = R C ] ) R A + R B = 100 kn
Problem 0. Three cables are attached as shown. Determine the reactions in the supports. Assume R B as redundant. Also, L AD L CD cos 60 m m. uation of uilibrium: + " Â F y 0 ) R A cos 60 + R B + R C cos
More information1.105 Solid Mechanics Laboratory Fall 2003 Experiment 3 The Tension Test
1.105 Solid Mechanics Laboratory Fall 2003 Experiment 3 The Tension Test Our objective is to measure the Elastic Modulus of steel. The experiment comes in two parts. In the first, you will subject a steel
More informationStrength of Material. Shear Strain. Dr. Attaullah Shah
Strength of Material Shear Strain Dr. Attaullah Shah Shear Strain TRIAXIAL DEFORMATION Poisson's Ratio Relationship Between E, G, and ν BIAXIAL DEFORMATION Bulk Modulus of Elasticity or Modulus of Volume
More informationMechanical Engineering Ph.D. Preliminary Qualifying Examination Solid Mechanics February 25, 2002
student personal identification (ID) number on each sheet. Do not write your name on any sheet. #1. A homogeneous, isotropic, linear elastic bar has rectangular cross sectional area A, modulus of elasticity
More informationModule III  Macromechanics of Lamina. Lecture 23. MacroMechanics of Lamina
Module III  Macromechanics of Lamina Lecture 23 MacroMechanics of Lamina For better understanding of the macromechanics of lamina, the knowledge of the material properties in essential. Therefore, the
More informationANALYSIS OF YARN BENDING BEHAVIOUR
ANALYSIS OF YARN BENDING BEHAVIOUR B. Cornelissen, R. Akkerman Faculty of Engineering Technology, University of Twente Drienerlolaan 5, P.O. Box 217; 7500 AE Enschede, the Netherlands b.cornelissen@utwente.nl
More informationANALYSIS OF YARN BENDING BEHAVIOUR
ANALYSIS OF YARN BENDING BEHAVIOUR B. Cornelissen, R. Akkerman Faculty of Engineering Technology, University of Twente Drienerlolaan 5, P.O. Box 217; 7500 AE Enschede, the Netherlands b.cornelissen@utwente.nl
More informationCHAPTER THREE SYMMETRIC BENDING OF CIRCLE PLATES
CHAPTER THREE SYMMETRIC BENDING OF CIRCLE PLATES * Governing equations in beam and plate bending ** Solution by superposition 1.1 From Beam Bending to Plate Bending 1.2 Governing Equations For Symmetric
More informationDEFORMATION PATTERN AND FAILURE CRITERIA OF WOVEN COMPOSITE PREFORM IN GENERAL BIAS EXTENSION
DEFORMATION PATTERN AND FAILURE CRITERIA OF WOVEN COMPOSITE PREFORM IN GENERAL BIAS EXTENSION B. Zhu 1,2*, T.X. Yu 1, X.M. Tao 2 1 Department of Mechanical Engineering, Hong Kong University of Science
More informationOperating Instructions For the Series Weavexx Tensometer Instrument
Operating Instructions For the 120000 Series Weavexx Tensometer Instrument Description The Weavexx Tensometer is a patented instrument for measuring tension in flexible, thin textile conveyor belts, paper,
More information1. A pure shear deformation is shown. The volume is unchanged. What is the strain tensor.
Elasticity Homework Problems 2014 Section 1. The Strain Tensor. 1. A pure shear deformation is shown. The volume is unchanged. What is the strain tensor. 2. Given a steel bar compressed with a deformation
More informationSTATICS. Friction VECTOR MECHANICS FOR ENGINEERS: Eighth Edition CHAPTER. Ferdinand P. Beer E. Russell Johnston, Jr.
Eighth E 8 Friction CHAPTER VECTOR MECHANICS FOR ENGINEERS: STATICS Ferdinand P. Beer E. Russell Johnston, Jr. Lecture Notes: J. Walt Oler Texas Tech University Contents Introduction Laws of Dry Friction.
More informationPES Institute of Technology
PES Institute of Technology Bangalore south campus, Bangalore5460100 Department of Mechanical Engineering Faculty name : Madhu M Date: 29/06/2012 SEM : 3 rd A SEC Subject : MECHANICS OF MATERIALS Subject
More informationTask 1  Material Testing of Bionax Pipe and Joints
Task 1  Material Testing of Bionax Pipe and Joints Submitted to: Jeff Phillips Western Regional Engineer IPEX Management, Inc. 20460 Duncan Way Langley, BC, Canada V3A 7A3 Ph: 6045348631 Fax: 6045347616
More informationEquilibrium. the linear momentum,, of the center of mass is constant
Equilibrium is the state of an object where: Equilibrium the linear momentum,, of the center of mass is constant Feb. 19, 2018 the angular momentum,, about the its center of mass, or any other point, is
More informationMECE 3321 MECHANICS OF SOLIDS CHAPTER 1
MECE 3321 MECHANICS O SOLIDS CHAPTER 1 Samantha Ramirez, MSE WHAT IS MECHANICS O MATERIALS? Rigid Bodies Statics Dynamics Mechanics Deformable Bodies Solids/Mech. Of Materials luids 1 WHAT IS MECHANICS
More information1 of 12. Given: Law of Cosines: C. Law of Sines: Stress = E = G
ES230 STRENGTH OF MATERIALS FINAL EXAM: WEDNESDAY, MAY 15 TH, 4PM TO 7PM, AEC200 Closed book. Calculator and writing supplies allowed. Protractor and compass required. 180 Minute Time Limit You must have
More informationElastic Properties of Solids Exercises I II for one weight Exercises III and IV give the second weight
Elastic properties of solids Page 1 of 8 Elastic Properties of Solids Exercises I II for one weight Exercises III and IV give the second weight This is a rare experiment where you will get points for breaking
More informationHigh Tech High Top Hat Technicians. An Introduction to Solid Mechanics. Is that supposed to bend there?
High Tech High Top Hat Technicians An Introduction to Solid Mechanics Or Is that supposed to bend there? Why don't we fall through the floor? The power of any Spring is in the same proportion with the
More informationINVESTIGATION OF THE PROCESSING PARAMETERS OF A 3D WOVEN REINFORCEMENT
INVESTIGATION OF THE PROCESSING PARAMETERS OF A 3D WOVEN REINFORCEMENT Andreas Endruweit, Dhiren K. Modi and Andrew C. Long School of Mechanical, Materials and Manufacturing Engineering, University of
More informationPurpose of this Guide: To thoroughly prepare students for the exact types of problems that will be on Exam 3.
ES230 STRENGTH OF MTERILS Exam 3 Study Guide Exam 3: Wednesday, March 8 th inclass Updated 3/3/17 Purpose of this Guide: To thoroughly prepare students for the exact types of problems that will be on
More informationUNIVERSITY OF SASKATCHEWAN ME MECHANICS OF MATERIALS I FINAL EXAM DECEMBER 13, 2008 Professor A. Dolovich
UNIVERSITY OF SASKATCHEWAN ME 313.3 MECHANICS OF MATERIALS I FINAL EXAM DECEMBER 13, 2008 Professor A. Dolovich A CLOSED BOOK EXAMINATION TIME: 3 HOURS For Marker s Use Only LAST NAME (printed): FIRST
More informationTHE LOSMANDY G11 MOUNT
Checking the parts THE LOSMANDY G11 MOUNT Depending on which accessories you ordered, your G11 mount was shipped in four or more boxes. The contents of each box are as follows: Equatorial Mount Adjustable
More informationStatics. Phys101 Lectures 19,20. Key points: The Conditions for static equilibrium Solving statics problems Stress and strain. Ref: 91,2,3,4,5.
Phys101 Lectures 19,20 Statics Key points: The Conditions for static equilibrium Solving statics problems Stress and strain Ref: 91,2,3,4,5. Page 1 The Conditions for Static Equilibrium An object in static
More informationPrediction of Draping Behavior of Woven Fabrics over DoubleCurvature Moulds Using Finite Element Techniques
International Journal of Material and Mechanical Engineering, 2012, 1: 2531  25  Published Online May 2012 http://www.ijmme.org Prediction of Draping Behavior of Woven Fabrics over DoubleCurvature
More informationLoad Washers. Force. for Forces of 7, kn. F z. Type 9001A A 9081B, 9091B
Force Load Washers for Forces of 7,5... 1 200 kn Type 9001A... 9071A 9081B, 9091B 1component force sensor for measuring dynamic and quasistatic forces in z direction. F z Calibrated measuring range 100
More informationLecture 8 Viscoelasticity and Deformation
Read: pg 130 168 (rest of Chpt. 4) 1 Poisson s Ratio, µ (pg. 115) Ratio of the strain in the direction perpendicular to the applied force to the strain in the direction of the applied force. For uniaxial
More informationQUESTION BANK SEMESTER: III SUBJECT NAME: MECHANICS OF SOLIDS
QUESTION BANK SEMESTER: III SUBJECT NAME: MECHANICS OF SOLIDS UNIT 1 STRESS AND STRAIN PART A (2 Marks) 1. Define longitudinal strain and lateral strain. 2. State Hooke s law. 3. Define modular ratio,
More informationVMSGeoMil. Background
Background When using a drilling rig for cone penetration testing, a mechanical clamp can be mounted to the drilling head (by means of a special transition piece). The depth than can be achieved depends
More informationPresented by: Civil Engineering Academy
Presented by: Civil Engineering Academy Structural Design and Material Properties of Steel Presented by: Civil Engineering Academy Advantages 1. High strength per unit length resulting in smaller dead
More informationDetermine the resultant internal loadings acting on the cross section at C of the beam shown in Fig. 1 4a.
E X M P L E 1.1 Determine the resultant internal loadings acting on the cross section at of the beam shown in Fig. 1 a. 70 N/m m 6 m Fig. 1 Support Reactions. This problem can be solved in the most direct
More informationSTRESS. Bar. ! Stress. ! Average Normal Stress in an Axially Loaded. ! Average Shear Stress. ! Allowable Stress. ! Design of Simple Connections
STRESS! Stress Evisdom! verage Normal Stress in an xially Loaded ar! verage Shear Stress! llowable Stress! Design of Simple onnections 1 Equilibrium of a Deformable ody ody Force w F R x w(s). D s y Support
More informationPrediction of fabric hand characteristics using extraction principle
Indian Journal of Fibre & Textile Research Vol. 41, March 2016, pp. 3339 Prediction of fabric hand characteristics using extraction principle Apurba Das a, Abhijit Majumdar & Sukumar Roy Department of
More informationTHEORETICAL DESIGN OF A NAILED OR BOLTED JOINT UNDER LATERAL LOAD 1. Summary
THEORETICAL DESIGN OF A NAILED OR BOLTED JOINT UNDER LATERAL LOAD 1 BY EDWARD W. KUENZI, 2 Engineer Forest Products Laboratory,3 Forest Service U. S. Department of Agriculture Summary This report presents
More informationChapter Two: Mechanical Properties of materials
Chapter Two: Mechanical Properties of materials Time : 16 Hours An important consideration in the choice of a material is the way it behave when subjected to force. The mechanical properties of a material
More informationINFLUENCE KINDS OF MATERIALS ON THE POISSON S RATIO OF WOVEN FABRICS
ISSN 18466168 (Print), ISSN 18485588 (Online) ID: TG217816142553 Original scientific paper INFLUENCE KINDS OF MATERIALS ON THE POISSON S RATIO OF WOVEN FABRICS Željko PENAVA, Diana ŠIMIĆ PENAVA, Željko
More informationThe University of Melbourne Engineering Mechanics
The University of Melbourne 436291 Engineering Mechanics Tutorial Four Poisson s Ratio and Axial Loading Part A (Introductory) 1. (Problem 922 from Hibbeler  Statics and Mechanics of Materials) A short
More informationQUESTION BANK DEPARTMENT: CIVIL SEMESTER: III SUBJECT CODE: CE2201 SUBJECT NAME: MECHANICS OF SOLIDS UNIT 1 STRESS AND STRAIN PART A
DEPARTMENT: CIVIL SUBJECT CODE: CE2201 QUESTION BANK SEMESTER: III SUBJECT NAME: MECHANICS OF SOLIDS UNIT 1 STRESS AND STRAIN PART A (2 Marks) 1. Define longitudinal strain and lateral strain. 2. State
More informationStatics Chapter II Fall 2018 Exercises Corresponding to Sections 2.1, 2.2, and 2.3
Statics Chapter II Fall 2018 Exercises Corresponding to Sections 2.1, 2.2, and 2.3 2 3 Determine the magnitude of the resultant force FR = F1 + F2 and its direction, measured counterclockwise from the
More informationRock Slope Analysis Small and Large Scale Failures Mode of Failure Marklands Test To establish the possibility of wedge failure. Plane failure is a special case of wedge failure. Sliding along
More informationDECLARATION. Supervised by: Prof Stephen Mutuli
DECLARATION The work presented in this project is the original work, which to the best of our knowledge has never been produced and presented elsewhere for academic purposes... EYSIMGOBANAY K. J F18/1857/006
More informationBIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS
BIAXIAL STRENGTH INVESTIGATION OF CFRP COMPOSITE LAMINATES BY USING CRUCIFORM SPECIMENS H. Kumazawa and T. Takatoya Airframes and Structures Group, Japan Aerospace Exploration Agency 6131, Ohsawa, Mitaka,
More informationDeflections and Strains in Cracked Shafts due to Rotating Loads: A Numerical and Experimental Analysis
Rotating Machinery, 10(4): 283 291, 2004 Copyright c Taylor & Francis Inc. ISSN: 1023621X print / 15423034 online DOI: 10.1080/10236210490447728 Deflections and Strains in Cracked Shafts due to Rotating
More informationExperimental Investigation of SoilPipe Friction Coefficients for Thermoplastic Pipes Installed in Selected Geological Materials
North American Society for Trenchless Technology (NASTT) NASTT s 2014 NoDig Show Orlando, Florida April 1317, 2014 MMT603 Experimental Investigation of SoilPipe Friction Coefficients for Thermoplastic
More information1 332 Laboratories 1. 2 Computational Exercises 1 FEA of a Cantilever Beam... 1 Experimental Laboratory: Tensile Testing of Materials...
1 332 Laboratories Contents 1 332 Laboratories 1 2 Computational Exercises 1 FEA of a Cantilever Beam.......................................... 1 Experimental Laboratory: Tensile Testing of Materials..........................
More informationMechanics of Solids. Mechanics Of Solids. Suraj kr. Ray Department of Civil Engineering
Mechanics Of Solids Suraj kr. Ray (surajjj2445@gmail.com) Department of Civil Engineering 1 Mechanics of Solids is a branch of applied mechanics that deals with the behaviour of solid bodies subjected
More informationInternational Journal of Scientific & Engineering Research, Volume 5, Issue 1, January ISSN
International Journal of Scientific & Engineering Research, Volume 5, Issue 1, January214 29 An Experimental Analysis of Stress Relaxation in Nonwoven Fabrics Sajid Ahmed Qureshi ABSTRACT  The current
More informationSTRESS, STRAIN AND DEFORMATION OF SOLIDS
VELAMMAL COLLEGE OF ENGINEERING AND TECHNOLOGY, MADURAI 625009 DEPARTMENT OF CIVIL ENGINEERING CE8301 STRENGTH OF MATERIALS I 
More informationME Final Exam. PROBLEM NO. 4 Part A (2 points max.) M (x) y. z (neutral axis) beam crosssec+on. 20 kip ft. 0.2 ft. 10 ft. 0.1 ft.
ME 323  Final Exam Name December 15, 2015 Instructor (circle) PROEM NO. 4 Part A (2 points max.) Krousgrill 11:30AM12:20PM Ghosh 2:303:20PM Gonzalez 12:301:20PM Zhao 4:305:20PM M (x) y 20 kip ft 0.2
More informationMAAE 2202 A. Come to the PASS workshop with your mock exam complete. During the workshop you can work with other students to review your work.
It is most beneficial to you to write this mock final exam UNDER EXAM CONDITIONS. This means: Complete the exam in 3 hours. Work on your own. Keep your textbook closed. Attempt every question. After the
More informationMechanics of Materials Primer
Mechanics of Materials rimer Notation: A = area (net = with holes, bearing = in contact, etc...) b = total width of material at a horizontal section d = diameter of a hole D = symbol for diameter E = modulus
More informationSimulation of Geometrical CrossSection for Practical Purposes
Simulation of Geometrical CrossSection for Practical Purposes Bhasker R.S. 1, Prasad R. K. 2, Kumar V. 3, Prasad P. 4 123 Department of Mechanical Engineering, R.D. Engineering College, Ghaziabad, UP,
More informationStructural Analysis Laboratory. Michael Storaker, Sam Davey and Rhys Witt. JEE 332 Structural Analysis. 4 June 2012.
Structural Analysis Laboratory Michael Storaker, Sam Davey and Rhys Witt JEE 332 Structural Analysis 4 June 2012 Lecturer/Tutor Shinsuke Matsuarbara 1 Contents Statically Indeterminate Structure Objective...
More informationINTRODUCTION TO STRAIN
SIMPLE STRAIN INTRODUCTION TO STRAIN In general terms, Strain is a geometric quantity that measures the deformation of a body. There are two types of strain: normal strain: characterizes dimensional changes,
More information3 Hours/100 Marks Seat No.
*17304* 17304 14115 3 Hours/100 Marks Seat No. Instructions : (1) All questions are compulsory. (2) Illustrate your answers with neat sketches wherever necessary. (3) Figures to the right indicate full
More informationLever Lab: First Class Lever
Lever Lab 2 Name: Lever Lab: First Class Lever Objective: To investigate the use of a lever as a simple machine. Materials: Workshop Stand, Lever, Bolt, Hooked Masses Background: A lever is one of the
More informationKey words: Polymeric Composite Bearing, Clearance, FEM
A study on the effect of the clearance on the contact stresses and kinematics of polymeric composite journal bearings under reciprocating sliding conditions Abstract The effect of the clearance on the
More informationAPI 11E  Specification for Pumping Units
API 11E  Specification for Pumping Units 5 Beam Pump Structure Requirements 5.1 General Requirements for beam pump structures are specified in the following sections. Only loads imposed on the structure
More informationA NEW CABLEPULLEY ALGORITHM IN RFEM
Journal of MECHANICAL ENGINEERING Strojnícky časopis Print ISSN 00392472 Online ISSN 24505471 VOLUME 66, NO 2, 2016 pp. 89 94 DOI:10.1515/scjme20160022 A NEW CABLEPULLEY ALGORITHM IN RFEM ŠTEKBAUER
More informationMEMS Project 2 Assignment. Design of a Shaft to Transmit Torque Between Two Pulleys
MEMS 029 Project 2 Assignment Design of a Shaft to Transmit Torque Between Two Pulleys Date: February 5, 206 Instructor: Dr. Stephen Ludwick Product Definition Shafts are incredibly important in order
More information2012 MECHANICS OF SOLIDS
R10 SET  1 II B.Tech II Semester, Regular Examinations, April 2012 MECHANICS OF SOLIDS (Com. to ME, AME, MM) Time: 3 hours Max. Marks: 75 Answer any FIVE Questions All Questions carry Equal Marks ~~~~~~~~~~~~~~~~~~~~~~
More informationCOURSE TITLE : APPLIED MECHANICS & STRENGTH OF MATERIALS COURSE CODE : 4017 COURSE CATEGORY : A PERIODS/WEEK : 6 PERIODS/ SEMESTER : 108 CREDITS : 5
COURSE TITLE : APPLIED MECHANICS & STRENGTH OF MATERIALS COURSE CODE : 4017 COURSE CATEGORY : A PERIODS/WEEK : 6 PERIODS/ SEMESTER : 108 CREDITS : 5 TIME SCHEDULE MODULE TOPICS PERIODS 1 Simple stresses
More informationIDE 110 Mechanics of Materials Spring 2006 Final Examination FOR GRADING ONLY
Spring 2006 Final Examination STUDENT S NAME (please print) STUDENT S SIGNATURE STUDENT NUMBER IDE 110 CLASS SECTION INSTRUCTOR S NAME Do not turn this page until instructed to start. Write your name on
More informationThe University of Melbourne Engineering Mechanics
The University of Melbourne 436291 Engineering Mechanics Tutorial Eleven Instantaneous Centre and General Motion Part A (Introductory) 1. (Problem 5/93 from Meriam and Kraige  Dynamics) For the instant
More informationMECHANICS OF MATERIALS. Prepared by Engr. John Paul Timola
MECHANICS OF MATERIALS Prepared by Engr. John Paul Timola Mechanics of materials branch of mechanics that studies the internal effects of stress and strain in a solid body. stress is associated with the
More informationParametric Study of Shaft Subjected To Pure Bending
Page167 Parametric Study of Shaft Subjected To Pure Bending Amar Kumar Patel*, Akash Kumar Patel**, Prajnasu Biswal***, & Satya Narayan Tripathy**** *Mechanical Department, Gandhi Institute of Engineering
More informationAdvanced Structural Analysis EGF Section Properties and Bending
Advanced Structural Analysis EGF316 3. Section Properties and Bending 3.1 Loads in beams When we analyse beams, we need to consider various types of loads acting on them, for example, axial forces, shear
More informationA FINITE ELEMENT MODEL TO PREDICT MULTI AXIAL STRESSSTRAIN RESPONSE OF CERAMIC MATRIX COMPOSITES WITH STRAIN INDUCED DAMAGE
A FINITE ELEMENT MODEL TO PREDICT MULTI AXIAL STRESSSTRAIN RESPONSE OF CERAMIC MATRIX COMPOSITES WITH STRAIN INDUCED DAMAGE Daxu Zhang and D. R. Hayhurst School of Mechanical, Aerospace and Civil Engineering,
More informationEMA 3702 Mechanics & Materials Science (Mechanics of Materials) Chapter 2 Stress & Strain  Axial Loading
MA 3702 Mechanics & Materials Science (Mechanics of Materials) Chapter 2 Stress & Strain  Axial Loading MA 3702 Mechanics & Materials Science Zhe Cheng (2018) 2 Stress & Strain  Axial Loading Statics
More information1 of 7. Law of Sines: Stress = E = G. Deformation due to Temperature: Δ
NME: ES30 STRENGTH OF MTERILS FINL EXM: FRIDY, MY 1 TH 4PM TO 7PM Closed book. Calculator and writing supplies allowed. Protractor and compass allowed. 180 Minute Time Limit GIVEN FORMULE: Law of Cosines:
More informationPLAT DAN CANGKANG (TKS 4219)
PLAT DAN CANGKANG (TKS 4219) SESI I: PLATES Dr.Eng. Achfas Zacoeb Dept. of Civil Engineering Brawijaya University INTRODUCTION Plates are straight, plane, twodimensional structural components of which
More informationAdvanced numerical modelling methods of rock bolt performance in underground mines
University of Wollongong Research Online Coal Operators' Conference Faculty of Engineering and Information Sciences 2010 Advanced numerical modelling methods of rock bolt performance in underground mines
More informationEng Sample Test 4
1. An adjustable tow bar connecting the tractor unit H with the landing gear J of a large aircraft is shown in the figure. Adjusting the height of the hook F at the end of the tow bar is accomplished by
More informationOn Nonlinear Buckling and Collapse Analysis using Riks Method
Visit the SIMULIA Resource Center for more customer examples. On Nonlinear Buckling and Collapse Analysis using Riks Method Mingxin Zhao, Ph.D. UOP, A Honeywell Company, 50 East Algonquin Road, Des Plaines,
More informationThe Relationship between the Applied Torque and Stresses in PostTension Structures
ECNDT 6  Poster 218 The Relationship between the Applied Torque and Stresses in PostTension Structures Fui Kiew LIEW, Sinin HAMDAN * and Mohd. Shahril OSMAN, Faculty of Engineering, Universiti Malaysia
More information